Application of magnetite nanomaterials for the removal of heavy metals from water.
Because access to safe drinking water is the key to protect public health, clean water has become a basic need of all properly functioning societies . Despite their presence at low concentration ranges, environmental pollutants possess serious threats to freshwater supply, living organisms, and public health .
Contamination of water with toxic metal ions (Hg(II), Pb(II), Cr(III), Cr(VI), Ni(II), Co(II), Cu(II), Cd(II), Ag(I), As(V) and As(III)) is becoming a severe environmental and public health problem. In order to achieve environmental detoxification, various techniques like adsorption, precipitation, ion exchange, reverse osmosis, electrochemical treatments, membrane filtration, evaporation, flotation, oxidation and biosorption processes are extensively used [3-5]. Among these, adsorption is a conventional but efficient technique to remove toxic metal ions and bacterial pathogens from water.
Development of novel and cost-effective nanomaterials for environmental remediation, pollution detection and other applications has attracted considerable attention. Recent advances suggest that many of the issues involving water quality could be resolved or greatly ameliorated using nanoparticles, nanofiltration or other products resulting from the development of nanotechnology [6-7].
The synthesis of magnetite nanoparticles has been intensively developed not only for its fundamental scientific interest but also for many technological applications: such as magnetic resonance imaging, ferrofluids for audio speakers, magnetic targeted drug delivery, and magnetic recording media . In particular, the use of magnetite nanoparticles as adsorbents in water treatment provides a convenient approach for separating and removing the contaminants by applying external magnetic fields.
Bare magnetite nanoparticles are susceptible to air oxidation and are easily aggregated in aqueous systems . Thus, for the application of these nanoparticles in various potential fields the stabilization of the iron oxide particles by surface modification is desirable. The magnetic structure of the surface layer, which is usually greatly different from that in the core of the nanoparticles, can have a notable effect on the magnetic properties of nanoparticles . The control of the size and the polydispersity are also very important because the properties of the nanocrystals strongly depend upon the dimension of the nanoparticles. It is interesting to mention that only magnetite particles with size of less than 30 nm have a large surface area and exhibit super paramagnetic properties that make them prone to magnetic fields and they do not become permanently magnetized without an external magnetic field to support them . These properties are highly useful in the development of novel separation processes .
To understand the behavior of the colloidal ferrofluids of the particles and to improve their applications or develop new ones, careful studies related to fluid stability, control of surfactants, particle sizes and physical behavior are essential .
We here present recent developments on the use of magnetite nanoparticles (NPs) and magnetite-containing composite nanomaterials for the removal of heavy metals from waters.
2. Synthesis of Fe3O4 nanoparticles
For different applications, several chemical methods can be used to synthesize magnetic nanoparticles: co-precipitation, reverse micelles and micro-emulsion technology, sol-gel syntheses, sonochemical reactions, hydrothermal reactions, hydrolysis and thermolysis of precursors, flow injection syntheses, and electrospray syntheses . The synthesis of superparamagnetic nanoparticles is a complex process because of their colloidal nature. For metal removal applications, an adequate surface modification of the nanoparticles is a critical aspect regarding both selectivity and aqueous stability of these materials. To this end, in the last decade, organic and inorganic functionalized Fe3O4 nanoparticles have been developed and modifications of the synthesis methods mentioned above have been proposed. A brief description of the methods most widely used for preparing materials with applications in metal removals is given below:
3. Characterization of Fe3O4 nanoparticles
Among the methods widely used in the literature for Fe3O4 nanoparticle characterization and surface determination are: Transmission Electron Microscopy (TEM), Scanning Electron Microscopy (SEM), Fourier Transform Infrared spectroscopy (FTIR), Powder X-ray Diffraction (XRD) Technique, Atomic Absorption Spectroscopy (AAS), Gel Permeation Chromatography (GPC), Differential Scanning Calorimetry (DSC), Thermogravimetric Analysis (TGA), Electrical Conductivity Measurement.
Among the methods used for the determination of the size and size distribution of nanoparticles, a few are applicable in various chemical environments, i.e. small-angle X-ray scattering (SAXS) and dynamic light scattering (DLS). One particular advantage of SAXS is that it can be used to analyze dispersions as well as powders or solids, whereas DLS is limited to dilute solutions. Comparing SAXS with an image-guided method like transmission electron microscopy (TEM), SAXS benefits from a higher statistical quality in the size distribution determination providing information about primary particles and aggregates from a single scattering experiment. Additionally, no high vacuum is required, which limits the samples to solid state samples. TEM has its specific benefits as it delivers direct images and local information on size and shape of nanoparticles. Therefore, these two techniques are complementary and combining both methods can lead to superior information with regard to shape and size of nanoparticles in dispersions or powders . A less common technique to obtain a particle size distribution is the analysis with nitrogen sorption. The evaluation according to BET theory (Brunauer–Emmet–Teller) allows obtaining information on the size of non-agglomerated and dense particles .
Comparison between the results obtained by the different techniques in the literature seem to support the view that comprehensive information on particle size, size distribution and shape require the use of more than one characterization technique. Each of the techniques has its specific advantages: TEM delivers direct images, from which information on size and shape of nanoparticles is obtained, SAXS is able to measure powders, solids and also particles in solution, DLS is a fast and cheap method to measure a high number of samples, and BET give the size of nanoparticles as a by-product from the main aim of the method, e.g. the determination of phases within a sample or the specific surface. For many nanomateriales it is observed that DLS exceeds SAXS and TEM by a factor of two or higher. Significantly larger values from DLS might be attributed to larger hydrodynamic shells, as a complex shape of particles as well as their aggregation can influence the numerical evaluation from DLS.
Powder XRD and electronic diffraction patterns (ED) are used to determine the crystal structure and characterization of the bulk Fe3O4 nanoparticles. Elemental analysis and surface coverage of magnetite particles may be measured by energy dispersive X-ray spectroscopy (SEM/EDS, EDAX). XPS is used for the analysis of the surface chemistry. Raman and Fourier transform infrared (FTIR) spectroscopy have been used to characterize the phase of the magnetic core of magnetite nanoparticles [28-29]. FTIR spectra yield information on the chemical bonds between the Fe3O4 core and the organic surface coverage .
Because of the peculiar magnetic properties of magnetite, the particles magnetization as a function of temperature and the hysteresis cycle of both magnetite and composite particles is also used for the characterization of the particle. Normally, magnetite nanoparticles exhibit overall magnetic behavior characteristic of soft magnetic particles, with a narrow hysteresis cycle, and a small coercive ﬁeld and remnant magnetization. The presence of nonmagnetic shells covering the nanoparticles is evidenced by the fact that magnetization is reduced compared to that of pure magnetite and the initial magnetization ﬁeld dependence is steeped in the latter case . In general, particle intrinsic coercivity (Hc) and the saturation magnetization are determined by vibrating sample magnetometer (VSM) . However, the effective magnetic core size of the particles may be measured by magnetic relaxometry (MRX) investigating the relaxation behavior in liquid suspensions .
Mössbauer spectroscopy analysis may also be performed to distinguish crystallographic phases . Magnetite particles exhibit ferromagnetic properties for observation times shorter than the relaxation time, while superparamagnetic properties are exhibited in the opposite case. Since the time of relaxation increases with the particle size, the Mössbauer spectrum of a dispersed system of magnetic nanocrystals is usually a superposition of a Zeeman sextet, corresponding to the large-size ferromagnetic particles, with a superparamagnetic doublet, corresponding to the particles of smaller size. However, since the time of relaxation in the system of interacting superparamagnetic particles can change due to correlation bonds arising between magnetization vectors of neighboring particles, the shape of the Mössbauer spectra depends both, on the inter-particle interaction and on the superparamagnetic properties of an individual particle. Therefore, interpretation of Mössbauer spectra yields information on particle size and on strong inter-particle interactions .
FTIR spectra yield information on the chemical bonds between the Fe3O4 core and the organic surface coverage .
Thermogravimetric and differential thermal analyses are essential for the determination of the weight of surfactant covering the particle surface per mass of magnetite, and for the determination of desorption binding heat of the covering layers [35-36].
Given that the surface properties of oxides are extremely sensitive to pH variations in the dispersion medium, determinations of the electrophoretic mobility and zeta-potential of the particles are also of importance for their technological applications .
4. Metal removal
In the present section we will describe recent literature results related to the application of magnetite nanomaterials for the removal of heavy metals and metalloids from water, mainly copper, chromium, mercury and arsenic.
Yantasee et al.  prepared superparamagnetic iron oxide (Fe3O4) nanoparticles with a surface functionalization of dimercaptosuccinic acid (DMSA) and employed them as an effective sorbent material for toxic soft metals such as Hg(II), Ag(I), Pb(II), Cd(II), and Tl(I) ions which effectively bind to the DMSA ligands and for As(III) which binds to the iron oxide lattices. The nanoparticles could be separated from solution within a minute with a 1.2 T magnet. The authors compared the chemical affinity, capacity, kinetics, and stability of the magnetic nanoparticles to those of conventional resin based sorbents (GT-73), activated carbon, and nanoporous silica (SAMMS) of similar surface chemistries in river water, groundwater, seawater, and human blood and plasma. DMSAFe3O4 showed a capacity of 227 mg of Hg/g, a 30-fold larger value than that of GT-73.
Singh et al  prepared magnetite nanoparticles functionalized with carboxyl (succinic acid), amine (ethylenediamine) and thiol (2,3-dimercaptosuccinic acid) groups These nanoparticles were used for removal of toxic metal ions (Cr(III), Co(II), Ni(II), Cu(II), Cd(II), Pb(II) and As(III)) and bacterial pathogens (Escherichia coli) from water.
Liu et al.  developed humic acid (HA) coated Fe3O4 nanoparticles (Fe3O4/HA) for the removal of toxic cations such as Hg(II), Pb(II), Cd(II), and Cu(II) from water. Fe3O4/HA were prepared by the coprecipitation method. TOC and XPS analyses showed that the as-prepared Fe3O4/HA contains ~11% (w/w) of HA fractions abundant in O and N-based functional groups. TEM images and laser particle size analysis revealed that the Fe3O4/HA (with ~10 nm Fe3O4 cores) aggregated in aqueous suspensions to form aggregates with an average hydrodynamic size of ~140 nm. Sorption of the heavy metals to Fe3O4/HA reached equilibrium in less than 15 min, and agreed well to the Langmuir adsorption model with maximum adsorption capacities ranging from 45 to 100 mg/g. The Fe3O4/HA was able to remove over 99% of Hg(II) and Pb(II), and over 95% of Cu(II) and Cd(II) in natural and tap water at optimized pH.
Badruddoza et al.  fabricated carboxymethyl-β-cyclodextrin modified Fe3O4 nanoparticles (CMβCD-MNPs) for removal of copper ions from aqueous solution by grafting CMβCD onto the magnetite surface via carbodiimide method. The characteristics results of FTIR, TEM, TGA and XPS show that CM-β-CD is grafted onto Fe3O4 nanoparticles. The grafted CM- β -CD on the Fe3O4 nanoparticles contributes to an enhancement of the adsorption capacity because of the strong abilities of the multiple hydroxyl and carboxyl groups in CM- β -CD to adsorb metal ions. The adsorption of Cu(II) onto CMCD-MNPs was found to be dependent on pH and temperature. The thermodynamic parameters reveal the feasibility, spontaneity and exothermic nature of the adsorption process. FTIR and XPS reveal that Cu(II) adsorption onto CMCD-MNPs mainly involves the oxygen atoms in CM-β-CD to form surface-complexes. In addition, the copper ions can be desorbed from CMCD-MNPs by citric acid solution with 96.2% desorption efficiency and the CMCD-MNPs exhibit good recyclability.
Goon et al.  studied the controlled adsorption of polyethylenimine (PEI) onto 50 nm crystalline magnetite nanoparticles (Fe3O4 NPs) and how these PEI-coated Fe3O4 NPs can be used for the magnetic capture and quantification of ultratrace levels of free cupric ions. The authors were able to systematically control the amount of PEI adsorbed onto the Fe3O4 magnetic nanoparticle surfaces by varying the concentration of polymer during the adsorption process. This work demonstrated that the NPs ability to bind with copper is highly dependent on the amount of PEI adsorbed on the NP surface. It was found that PEI-coated Fe3O4 NPs were able to capture trace levels (~2 ppb) of free cupric ions and concentrate the ions to allow for detection via ICP-OES. They also showed that due to the amine-rich structure of PEI, the PEI-coated Fe3O4 NPs selectively adsorb toxic free cupric ions but not the less toxic EDTA complexed copper.
Chou and Lien  prepared dendrimer-conjugated magnetic nanoparticles (Gn-MNPs) combining the superior adsorbent of dendrimers with magnetic nanoparticles (MNPs) for effective removal and recovery of Zn(II). The adsorption efficiency increases with increasing pH. At pH less than 3, Zn(II) is readily desorbed. Hence, the Gn-MNPs can be regenerated using a diluted HCl aqueous solution (0.1 M) and Zn(II) can be recovered in a concentrated form. It was found that the Gn-MNPs still retained the original removal capacity of Zn(II) after 10 consecutive adsorption–desorption stages.
Wang et al.  developed amino-functionalized Fe3O4@SiO2 magnetic nanomaterial with a core–shell structure to remove heavy metal ions from aqueous media. The structural, surface, and magnetic characteristics of the nanosized adsorbent were investigated by elemental analysis, FTIR, N2 adsorption–desorption, transmission electron microscopy, powder X-ray diffraction, X-ray photoelectron spectroscopy, vibrating sample magnetometry, thermogravimetric analysis, and zeta-potential measurement. The amino-functionalized Fe3O4@SiO2 nanoadsorbent exhibited high adsorption affinity for aqueous Cu(II), Pb(II), and Cd(II) ions, resulting from complexation of the metal ions by surface amino groups. Moreover, the adsorption affinity for heavy metal ions was not much affected by the presence of a cosolute of humic acid or alkali/earth metal ions (Na+, K+, etc.). The metal-loaded Fe3O4@SiO2–NH2 nanoparticles could be recovered readily from aqueous solution by magnetic separation and regenerated easily by acid treatment.
Shishehbore et al.  reported a method for the pre-concentration of trace heavy metal ions in environmental samples. The method is based on the sorption of Cu(II), Cd(II), Ni(II) and Cr(III) ions with salicylic acid as chelate on silica-coated magnetite nanoparticles. The adsorbent was characterized by XRD, SEM, BET and FT-IR measurements. The method was successfully applied to the evaluation of these trace and toxic metals in various waters, foods and other samples.
Wu et al.  showed that Fe3O4 can be used to disperse nano-Fe0 and thus sustain Cr(VI) mitigation by nano-Fe0. Fe0 nanoparticles can attach to the surface of Fe3O4 by addition of large Fe3O4-NPs into the reaction solution during the preparation of Fe0 nanoparticles. The introduction of Fe3O4 prevents the aggregation of Fe0 nanoparticles and keeps the high efficiency of the nanocomposite for Cr(VI) reduction. Their results suggest that higher proportions of Fe3O4 in the nanocomposites could increase the rate of Cr(VI) reduction, and the optimal ratio of Fe3O4:Fe0 for Cr(VI) reduction was determined to be 40:1. The authors also showed that solution pHs significantly affect the rate of Cr(VI) reduction, with reactions occurring faster under acidic or neutral than basic conditions.
Cutting et al.  showed that nanomagnetites produced by the bacterial reduction of schwertmannite powder were more efficient at reducing Cr(VI) than either ferrihydrite “gel”-derived biomagnetite or commercial nanoscale Fe3O4. Schwertmannite-derived biomagnetite proved capable of retaining more (~20%) 99mTc(VII) than ferrihydrite-derived biomagnetite, confirming that the production of biomagnetite can be fine-tuned for efficient environmental remediation through careful selection of the Fe(III) mineral substrate supplied to Fe(III)-reducing bacteria.
Wang et al.  investigated As(V) speciation resulting from different sorption processes on magnetite nanoparticles, including both adsorption and precipitation. Using X-ray absorption fine structure (XAFS) spectroscopy and transmission electron microscopy (TEM), they conclude that As(V) could form complexes at the surfaces of the small nanoparticles and could be progressively incorporated in their structure with increasing As loading. These results provide some of the fundamental knowledge about As(V)-magnetite interactions that is essential for developing effective water treatment technologies for arsenic.
Chen et al.  synthesized multiwalled boron nitride nanotubes (BNNTs) functionalized with Fe3O4 nanoparticles (NPs) for arsenic removal from water solutions. Adsorption experiments conducted at neutral pH (6.9) and room temperature using the developed nanocomposites revealed effective arsenic (V) removal. The Langmuir, Freundlich, and Dubinin-Radushkevich adsorption isotherms were tested for a range of As(V) initial concentrations from 1 to 40 mg/L under the same conditions. The equilibrium data well fitted all isotherms, indicating that the mechanism for As(V) adsorption was a combination of chemical complexation and physical electrostatic attraction with a slight preference for chemisorption.
Chowdhury and Yanful  investigated the adsorption of arsenic and chromium by mixed magnetite and maghemite nanoparticles from aqueous solution. These authors employed a commercially grade nanosize ‘magnetite’, later identified in laboratory characterization to be mixed magnetite-maghemite nanoparticles in the uptake of arsenic and chromium from different water samples. Their results showed 96-99% arsenic and chromium uptake under controlled pH conditions. The maximum arsenic adsorption occurred at pH 2 with values of 3.69 mg/g for As(III) and 3.71 mg/g for As(V) when the initial concentration was kept at 1.5 mg/L for both arsenic species, while at the same pH Cr(VI) sorption capacity was 2.4 mg/g with an initial Cr(VI) concentration of 1 mg/L. Their results also showed the limitation of arsenic and chromium uptake by the nano-size magnetite-maghemite mixture in the presence of a competing anion such as phosphate.
Yang et al.  studied the effect of Zn(II) on both the kinetic and equilibrium behavior of arsenic adsorption to magnetite nanoparticles in the pH range 4.5-8.0. At pH 8.0, adsorption of both arsenate and arsenite to magnetite nanoparticles was significantly enhanced by the presence of small amount of Zn(II) in the solution. The adsorption rate also increased significantly in the presence of Zn(II). The adsorption enhancement effect of Zn(II) was not observed at pH 4.5-6.0, nor with ZnO nanoparticles, nor with surface-coated Zn-magnetite nanoparticles. The enhanced arsenic adsorption in the presence of Zn(II) cannot be due to reduced negative charge of the magnetite nanoparticles surface by adsorption of Zn(II) because other cations, such as Ca(II) and Ag(I), failed to enhance arsenic adsorption. Formation of a ternary surface complex by zinc, arsenic and magnetite nanoparticles was proposed as a possible mechanism controlling the observed zinc effect. Zinc-facilitated adsorption provides further advantage for magnetite nanoparticle-enhanced arsenic removal over conventional treatment approaches.
Zhang et al.  showed that the application of starch as a stabilizer in preparation of the Fe3O4 particles is able to efficiently reduce particle aggregation, and thus, effective particle size, resulting in much greater specific surface area and adsorption sites. Moreover, the presence of starch leads to the formation of more effective adsorbing sites on magnetite particle surfaces. By employing the XAFS technique, the authors showed that arsenate is adsorbed on starch-stabilized magnetite nanoparticles mainly as inner-sphere bidentate and monodentate complexes. The coordination numbers of As-Fe binding increases with increasing starch concentration, which indicates that the arsenate is more firmly adsorbed at higher starch concentrations.
An et al.  prepared and tested a new class of starch-bridged magnetite nanoparticles for removal of arsenate from spent ion exchange brine. Maximum uptake was observed within a pH range of 4-6. The Langmuir capacity coefficient was determined to be 248 mg/g at pH 5.0. The final treatment sludge was able to pass the TCLP (Toxicity Characteristic Leaching Procedure) based leachability of 5 mg/L as As.
All the results described in this section are summarized in Table 1.
As illustrated in this book chapter, the use of magnetite nanoparticles as adsorbents in water treatment provides a convenient approach for separating and removing the contaminants by applying external magnetic fields. In particular, technologies based on the utilization of magnetite nanoparticles for the removal of heavy metals from wastewaters are under active development as highly effective, efficient and economically viable nanoadsorbents. Among the main advantages of these nanomaterials is the possibility of surface modifications with different organic or inorganic coating agents to allow the removal of a wide range of heavy metals with specificity. However, the application of these methods is still limited in the early stage and more research in the field is certainly necessary.
In conclusion, there is much recent interest in the use of engineered magnetite nanoparticles in wastewater treatment. However, uncertainties over the health impacts and environmental fate of these nanomaterials need to be addressed before their widespread application. Research on their fate and impact in the environment is required due to the discharges already occurring to the environment.
|Thermolysis of precursors||dimercaptosuccinic acid||Thiol group||Hg(II), Ag(I), Pb(II), Cd(II), Tl+|||
|Co-precipitation||succinic acid||Carboxylic group||Cr(III), Co(II), Ni(II), Cu(II), Cd(II), Pb(II), As(III)||
|Thermolysis of precursors||ethylenediamine||Amine group|
|Thermolysis of precursors followed by ligand exchange process||dimercaptosuccinic acid||Thiol group|
|Co-precipitation||Humic acid||Carboxylic and phenolic group||Hg(II), Pb(II), Cd(II), Cu(II)|||
|Crystallization from ferrous hydroxide gels||polyethylenimine||Amine group||Cu(II)|||
|Co-precipitation followed by a sol-gel process using sodium silicate (Fe3O4@SiO2)||(3-aminopropyl) trimethoxysilane||Amine group||Pb(II), Cd(II), Cu(II)|||
|Co-precipitation followed by hydrolysis of TEOS, (Fe3O4@SiO2)||salicylic acid functionalized silica||Carboxylic group||Cu(II), Cd(II), Ni(II), Cr(III)|||
|Stabilization of Fe0 nanoparticles with Fe3O4||-||-||Cr(VI)|||
|Bacterial reduction of schwertmannite||-||-||Cr(VI), Tc(VII)|||
|BNNTs functionalized with Fe3O4 nanoparticles||-||-||As(V)|||
|Commercially available magnetite-maghemite mixture nanoparticles||-||-||As(V), As(III), Cr(VI)|||
|Commercially available magnetite.||-||-||As(V), As(III)|||
|Modification of co-precipitation method||Starch||hydroxyl group||As(V)|||
|Modification of co-precipitation method||Starch||hydroxyl group||As(V)|||
World Health Organization, Guidelines for Drinking-water Quality, 3rd Edition, Incorporating the first and second addenda, Vol. 1, Recommendations, Geneva, Switzerland. Retrieved from http://www.who.int/water_sanitation_health/dwq/fulltext.pdf, (2008).
P.L. Brezonik and W.A. Arnold, Water chemistry: Fifty years of change and progress, Environmental Science and Technology 46 (2012) 5650-5657.
S. Chen, Y. Zou, Z. Yan, W. Shen, S. Shi, X. Zhang and H. Wang, Carboxymethylated-bacterial cellulose for copper and lead ion removal, Journal of Hazardous Materials 161 (2009) 1355-1359.
Y. Chen, B. Pan, H. Li, W. Zhang, L. Lv and J. Wu, Selective removal of Cu(II) ions by using cation-exchange resin-supported polyethyleneimine (PEI) nanoclusters, Environmental Science and Technology 44 (2010) 3508-3513.
V. Ivanov, J.H. Tay, S.T.L. Tay and H.L. Jiang, Removal of micro-particles by microbial granules used for aerobic wastewater treatment Water Science and Technology 50 (2004) 147-154.
J. Schulte and J. Dutta, Nanotechnology in environmental protection and pollution, Science and Technology of Advanced Materials 6 (2005) 219-220.
M. Auffan, H.J. Shipley, S. Yean, A.T. Kan, M. Tomson, J. Rose and J.Y. Bottero, Nanomaterials as adsobents, in: M.R. Wiesner, J.Y. Bottero (Eds), Environmental Nanotechnology: Applications and Impacts of Nanomaterials, McGraw-Hill, New York (2007) 371-392.
S. Laurent, D. Forge, M. Port, A. Roch, C. Robic, L. Vander Elst and R.N. Muller, Magnetic iron oxide nanoparticles: Synthesis, stabilization, vectorization, physicochemical characterizations and biological applications, Chemical Reviews 108 (2008) 2064-2110.
D. Maity and D.C. Agrawal, Synthesis of iron oxide nanoparticles under oxidizing environment and their stabilization in aqueous and non-aqueous media, Journal of Magnetism and Magnetic Materials 308 (2007) 46-55.
L. Zhang, R. He and H.C. Gu, Oleic acid coating on the monodisperse magnetite nanoparticles, Applied Surface Science 253 (2006) 2611-2617.
Y.T. Zhou, H.L. Nie, C. Branford-White, Z.Y. He and L.M. Zhu, Removal of Cu2+ from aqueous solution by chitosan-coated magnetic nanoparticles modified with α-ketoglutaric acid, Journal of Colloid and Interface Science 330 (2009) 29-37.
W. Yantasee, C.L. Warner, T. Sangvanich, R.S. Addleman, T.G. Carter, R.J. Wiacek, G.E. Fryxell, C. Timchalk and M.G. Warner, Removal of heavy metals from aqueous systems with thiol functionalized superparamagnetic nanoparticles, Environmental Science and Technology 41 (2007) 5114-5119.
H.C. Schwarzer and W. Peukert, Tailoring particle size through nanoparticle precipitation, Chemical Engineering Communications 191 (2004) 580-606.
J.P. Jolivet, C. Chanéac and E. Tronc, Iron oxide chemistry. From molecular clusters to extended solid networks, Chemical Communications 10 (2004) 481-487.
M.P. Pileni and N. Duxin, Micelle technology for magnetic nanosized alloys and composites, Chemical Innovation 30 (2000) 25-33.
Y. Deng, L. Wang, W. Yang, S. Fu and A. Elaïssari, Preparation of magnetic polymeric particles via inverse microemulsion polymerization process, Journal of Magnetism and Magnetic Materials 257 (2003) 69-78.
S. Sun and H. Zeng, Size-controlled synthesis of magnetite nanoparticles, Journal of the American Chemical Society 124 (2002) 8204-8205.
T.J. Daou, G. Pourroy, S. Bégin-Colin, J.M. Grenèche, C. Ulhaq-Bouillet, P. Legaré, P. Bernhardt, C. Leuvrey and G. Rogez, Hydrothermal synthesis of monodisperse magnetite nanoparticles, Chemistry of Materials 18 (2006) 4399-4404.
J. Wang, Z. Peng, Y. Huang and Q. Chen, Growth of magnetite nanorods along its easy-magnetization axis of [1 1 0], Journal of Crystal Growth 263 (2004) 616-619.
N. Mizutani, T. Iwasaki, S. Watano, T. Yanagida, H. Tanaka and T. Kawai, Effect of ferrous/ferric ions molar ratio on reaction mechanism for hydrothermal synthesis of magnetite nanoparticles, Bulletin of Materials Science 31 (2008) 713-717.
J. Du and C. Jing, Preparation of Fe3O4@Ag SERS substrate and its application in environmental Cr(VI) analysis, Journal of Colloid and Interface Science 358 (2011) 54-61.
M. Chen, S. Yamamuro, D. Farrell and S.A. Majetich, Gold-coated iron nanoparticles for biomedical applications, Journal of Applied Physics 93 (2003) 7551-7553.
R. Fu, X. Jin, J. Liang, W. Zheng, J. Zhuang and W. Yang, Preparation of nearly monodispersed Fe3O4/SiO2 composite particles from aggregates of Fe3O4 nanoparticles, Journal of Materials Chemistry 21 (2011) 15352-15356.
P. Mulvaney, L.M. Liz-Marzán, M. Giersig and T. Ung, Silica encapsulation of quantum dots and metal clusters, Journal of Materials Chemistry 10 (2000) 1259-1270.
C.F. Chang, Y.L. Wu and S.S. Hou, Preparation and characterization of superparamagnetic nanocomposites of aluminosilicate/silica/magnetite, Colloids and Surfaces A: Physicochemical and Engineering Aspects 336 (2009) 159-166.
S. Pabisch, B. Feichtenschlager, G. Kickelbick and H. Peterlik, Effect of interparticle interactions on size determination of zirconia and silica based systems - A comparison of SAXS, DLS, BET, XRD and TEM, Chemical Physics Letters 521 (2012) 91-97.
H.K. Kammler, G. Beaucage, R. Mueller and S.E. Pratsinis, Structure of flame-made silica nanoparticles by ultra-small-angle x-ray scattering, Langmuir 20 (2004) 1915-1921.
C. Galindo-Gonzalez, J.M. Feinberg, T. Kasama, L.C. Gontard, M. Pósfai, I. Kósa, J.D.G. Duran, J.E. Gil, R.J. Harrison and R.E. Dunin-Borkowski, Magnetic and microscopic characterization of magnetite nanoparticles adhered to clay surfaces, American Mineralogist 94 (2009) 1120-1129.
L. Slavov, M.V. Abrashev, T. Merodiiska, C. Gelev, R.E. Vandenberghe, I. Markova-Deneva and I. Nedkov, Raman spectroscopy investigation of magnetite nanoparticles in ferrofluids, Journal of Magnetism and Magnetic Materials 322 (2010) 1904-1911.
P. Russo, D. Acierno, M. Palomba, G. Carotenuto, R. Rosa, A. Rizzuti and C. Leonelli, Ultrafine magnetite nanopowder: Synthesis, characterization, and preliminary use as filler of polymethylmethacrylate nanocomposites, Journal of Nanotechnology (2012).
S.A. Gómez-Lopera, R.C. Plaza and A.V. Delgado, Synthesis and characterization of spherical magnetite/biodegradable polymer composite particles, Journal of Colloid and Interface Science 240 (2001) 40-47.
S. Beyaz, H. Kockar and T. Tanrisever, Simple synthesis of superparamagnetic magnetite nanoparticles and ion effect on magnetic fluids, Journal of Optoelectronics and Advanced Materials 1 (2009) 447 - 450.
B. Gleich and J. Weizenecker, Tomographic imaging using the nonlinear response of magnetic particles, Nature 435 (2005) 1214-1217.
M. Polikarpov, V. Cherepanov, M. Chuev, S. Shishkov and S. Yakimov, Mössbauer spectra of hematite and magnetite nanoparticles in polymer composites, Journal of Physics: Conference Series 217 (2010).
Y. Sahoo, H. Pizem, T. Fried, D. Golodnitsky, L. Burstein, C.N. Sukenik and G. Markovich, Alkyl phosphonate/phosphate coating on magnetite nanoparticles: A comparison with fatty acids, Langmuir 17 (2001) 7907-7911.
M. Mahmoudi, A. Simchi, M. Imani, A.S. Milani and P. Stroeve, Optimal design and characterization of superparamagnetic iron oxide nanoparticles coated with polyvinyl alcohol for targeted delivery and imaging, Journal of Physical Chemistry B 112 (2008) 14470-14481.
S. Singh, K.C. Barick and D. Bahadur, Surface engineered magnetic nanoparticles for removal of toxic metal ions and bacterial pathogens, Journal of Hazardous Materials 192 (2011) 1539-1547.
J.F. Liu, Z.S. Zhao and G.B. Jiang, Coating Fe3O4 Magnetic Nanoparticles with Humic Acid for High Efficient Removal of Heavy Metals in Water, Environmental Science & Technology 42 (2008) 6949-6954.
A.Z.M. Badruddoza, A.S.H. Tay, P.Y. Tan, K. Hidajat and M.S. Uddin, Carboxymethyl-β-cyclodextrin conjugated magnetic nanoparticles as nano-adsorbents for removal of copper ions: Synthesis and adsorption studies, Journal of Hazardous Materials 185 (2011) 1177-1186.
I.Y. Goon, C. Zhang, M. Lim, J.J. Gooding and R. Amal, Controlled fabrication of polyethylenimine-functionalized magnetic nanoparticles for the sequestration and quantification of free Cu2+, Langmuir 26 (2010) 12247-12252.
C.M. Chou and H.L. Lien, Dendrimer-conjugated magnetic nanoparticles for removal of zinc (II) from aqueous solutions, Journal of Nanoparticle Research 13 (2011) 2099-2107.
J. Wang, S. Zheng, Y. Shao, J. Liu, Z. Xu and D. Zhu, Amino-functionalized Fe3O4@SiO2 core-shell magnetic nanomaterial as a novel adsorbent for aqueous heavy metals removal, Journal of Colloid and Interface Science 349 (2010) 293-299.
M.R. Shishehbore, A. Afkhami and H. Bagheri, Salicylic acid functionalized silica-coated magnetite nanoparticles for solid phase extraction and preconcentration of some heavy metal ions from various real samples, Chemistry Central Journal 5 (2011).
Y. Wu, J. Zhang, Y. Tong and X. Xu, Chromium (VI) reduction in aqueous solutions by Fe3O4-stabilized Fe0 nanoparticles, Journal of Hazardous Materials 172 (2009) 1640-1645.
R.S. Cutting, V.S. Coker, N.D. Telling, R.L. Kimber, C.I. Pearce, B.L. Ellis, R.S. Lawson, D.E.R. Van Gerrit Laan, R.A.D. Pattrick, D.J. Vaughan, E. Arenholz and J.R. Lloyd, Optimizing Cr(VI) and Tc(VII) Remediation through Nanoscale Biomineral Engineering, Environmental Science and Technology 44 (2010) 2577-2584.
Y. Wang, G. Morin, G. Ona-Nguema, F. Juillot, G. Calas and G.E. Brown, Distinctive arsenic(V) trapping modes by magnetite nanoparticles induced by different sorption processes, Environmental Science and Technology 45 (2011) 7258-7266.
R. Chen, C. Zhi, H. Yang, Y. Bando, Z. Zhang, N. Sugiur and D. Golberg, Arsenic (V) adsorption on Fe3O4 nanoparticle-coated boron nitride nanotubes, Journal of Colloid and Interface Science 359 (2011) 261-268.
S.R. Chowdhury and E.K. Yanful, Arsenic and chromium removal by mixed magnetite-maghemite nanoparticles and the effect of phosphate on removal, Journal of Environmental Management 91 (2010) 2238-2247.
W. Yang, A.T. Kan, W. Chen and M.B. Tomson, PH-dependent effect of zinc on arsenic adsorption to magnetite nanoparticles, Water Research 44 (2010) 5693-5701.
M. Zhang, G. Pan, D. Zhao and G. He, XAFS study of starch-stabilized magnetite nanoparticles and surface speciation of arsenate, Environmental Pollution 159 (2011) 3509-3514.
B. An, Q. Liang and D. Zhao, Removal of arsenic(V) from spent ion exchange brine using a new class of starch-bridged magnetite nanoparticles, Water Research 45 (2011) 1961-1972.